**Graphene **

**Nanoplasmonics **

### Paulo André Dias Gonçalves

Mestrado em Física

Departamento de Física e Astronomia 2014

**Orientador **

Nuno Miguel Machado Reis Peres, Professor Catedrático, Escola de Ciências da Universidade do Minho

**Coorientador **

João Manuel Borregana Lopes dos Santos, Professor

Todas as correções determinadas pelo júri, e só essas, foram efetuadas.

O Presidente do Júri,

### Graphene Nanoplasmonics

### Paulo Andr´

### e Dias Gon¸

### calves

### Departamento de F´ısica e Astronomia

### Faculdade de Ciˆ

### encias da Universidade do Porto

### Porto, 2014

### Paulo Andr´

### e Dias Gon¸

### calves

### Graphene Nanoplasmonics

Thesis submitted to the Faculdade de Ciˆencias da Universidade do Porto in partial fulfillment of the requirements for the degree of Master in Physics

Departamento de F´ısica e Astronomia Faculdade de Ciˆencias da Universidade do Porto

i

“Science knows no country, because knowledge belongs to humanity, and is the torch which illuminates the world”.

### Acknowledgments

First of all, I would like to thank my advisors, professor Nuno Peres and professor Jo˜ao Lopes dos Santos for guiding me through this journey. I could not have asked for better tutors, whose invaluable knowledge and enthusiasm about physics I will never forget. In particular, I must offer my sincerest gratitude to professor Nuno Peres, for his continuous support, patience and inspiring dedication. I will always be grateful to have had the opportunity to work with you.

Additionally, I want to acknowledge all the colleagues and friends whom I had the priviledge to meet during my MSc studies at FCUP. Special thanks to Artur Amorim for all the amusing lunches talking about physics and the simple joys of life. Likewise, many thanks to Nuno Rodrigues for his friend-ship and relaxing conversations.

Furthermore, I would like to express my gratitude towards professor Jos´e Carlos Gomes, F´abio Hip´olito, and all the people at the Graphene Research Centre in Singapore, for their hospitality and all the good times we have spent during my research stay in Singapore.

Finally, I must thank my parents, brother and grandparents for their af-fection and for always being there for me. Last, but not least, I am thankful to Inˆes for her unconditional love, kindness and wholehearted support.

I acknowledge the Calouste Gulbenkian Foundation for finacial support through grant “Pr´emio Est´ımulo `a Investiga¸c˜ao 2013 ”, No. 132394.

### Resumo

Nos ´ultimos anos, a plasm´onica em grafeno tem recebido uma elevada aten¸c˜ao por parte da comunidade cient´ıfica. Esta ´area ainda jovem mas em r´apido crescimento, que resulta da sobreposi¸c˜ao entre a f´ısica do grafeno e a plas-m´onica, centra-se no estudo e explora¸c˜ao de plasm˜oes-polarit˜oes de superf´ıcie suportados pelo grafeno (graphene surface plasmon-polaritons) (GSPs) com o intuito de controlar interac¸c˜oes luz-mat´eria e manipular radia¸c˜ao electro-magn´etica `a nanoescala.

Nesta tese, depois de introduzirmos os conceitos elementares em plas-m´onica baseada em metais, procedemos `a deriva¸c˜ao da rela¸c˜ao de dispers˜ao de GSPs tranversos magn´eticos (TM) numa monocamada de grafeno. O espectro plasm´onico ´e primeiramente calculado numericamente, sendo pos-teriormente obtido por meios anal´ıticos em alguns casos limites, aos quais se segue a defini¸c˜ao de quantidades f´ısicas relevantes como o comprimento de propaga¸c˜ao dos GSPs a o grau de confinamento dos respectivos campos electromagn´eticos. Resultados semelhantes s˜ao tamb´em apresentados para o caso de uma dupla camada de grafeno; neste caso, devido `a intera¸c˜ao de Coulomb inter-camada entre GSPs em diferentes folhas de grafeno, a rela¸c˜ao de dispers˜ao correspondente consiste em dois ramos: um plasm˜ao ´optico com dispers˜ao tipo ra´ız quadrada e um ramo ac´ustico com dispers˜ao linear. De modo a acoplar GSPs a radia¸c˜ao electromagn´etica propagante, revemos tam-b´em as t´ecnicas mais comuns para excitar GSPs. Acresce, ainda, o estudo te´orico do lan¸camento de GSPs por um contacto met´alico colocado sobre uma folha de grafeno, motivado por um trabalho experimental recente. Fi-nalmente, ´e apresentada uma descri¸c˜ao detalhada da f´ısica fundamental sub-jacente `a excita¸c˜ao de GSPs numa estrutura peri´odica composta por fitas de

vi

grafeno, bem como a sua dependˆencia em v´arios parˆametros. De seguida, os resultados te´oricos obtidos usando o modelo anal´ıtico desenvolvido s˜ao com-parados com os resultados experimentais publicados na literatura, tendo-se obtido um acordo not´avel entre teoria e experiˆencia.

### Abstract

Over the last few years, graphene plasmonics has been receiving a lot of attention from the scientific community. This still young but rapidly growing field, resulting from the overlap between graphene physics and plasmonics, deals with the investigation and exploitation of graphene surface plasmon-polaritons (GSPs) for controlling light-matter interactions and manipulating light at the nanoscale.

In this thesis, after introducing the elementary concepts in conventional metal-based plasmonics, we move on to the derivation of the dispersion rela-tion of transverse magnetic (TM) GSPs in single-layer graphene. The plas-monic spectrum is first computed numerically and then obtained analytically in some limiting cases, followed by the definition of relevant quantities such as GSP propagation length and a measure of the degree of field confinement. Similar results are also presented for double-layer graphene; in this case, due to the inter-layer Coulomb interaction among GSPs in different graphene sheets, the corresponding dispersion relation consists in two branches: one optical plasmon with square-root dispersion and one acoustic branch with linear dispersion. We also briefly review the most common techniques for effectively exciting GSPs, since they cannot couple directly to free propa-gating electromagnetic waves. Further, motivated by a recent experimental work, we theoretically study the launching of GSPs by a metallic contact placed on top of monolayer graphene. Finally, a detailed discussion of the physics underlying GSPs excitations in a periodic array of graphene ribbons is presented, and the dependence of the GSP-induced absorption peak on a wide range of parameters is investigated. We then compare the theoretical results yielded by our analytical framework against available experimental

viii

data, having achieved a remarkable agreement between theory and experi-ment.

### Contents

Acknowledgments iii

Resumo v

Abstract vii

List of Figures xiv

List of Acronyms xv

1 Introduction 1

1.1 Context . . . 1

1.2 Structure of this thesis . . . 4

2 Electromagnetic Properties of Solids 7 2.1 Classical Electrodynamics . . . 7

2.1.1 Maxwell’s equations . . . 8

2.1.2 Boundary conditions . . . 11

2.2 Drude Model . . . 11

2.3 Graphene for Plasmonics . . . 13

2.3.1 Optical conductivity of graphene . . . 14

3 Surface Plasmon Polaritons at Dielectric-Metal Interfaces 17 3.1 Single Dielectric-Metal Interface . . . 17

3.1.1 Dispersion relation . . . 18

x CONTENTS

3.2 Multilayer Structures: Double Interface . . . 29

3.2.1 Dispersion relation . . . 30

4 Graphene Surface Plasmons 39 4.1 Monolayer Graphene . . . 40

4.1.1 Spectrum of TM GSPs . . . 40

4.1.2 Field profile of GSPs in single-layer graphene . . . 48

4.1.3 A word on TE GSPs . . . 51

4.2 Double-Layer Graphene . . . 52

4.2.1 Dispersion relation . . . 53

4.2.2 Field profile of GSPs in double-layer graphene . . . 57

5 Excitation of Graphene Surface Plasmons 61 5.1 Grating Coupling . . . 61

5.2 Prism Coupling . . . 62

5.3 Near-field Excitation and Imaging of GSPs . . . 64

5.4 Others . . . 66

6 Launching Plasmons using a Metal Contact 67 7 Plasmonics in Periodic Graphene-based Structures 81 7.1 Theoretical Model . . . 82

7.1.1 Setting up the model . . . 82

7.1.2 The scattering problem . . . 85

7.2 Applications and Results . . . 87

7.2.1 Periodic array of graphene ribbons . . . 87

7.2.2 Theory versus experiment . . . 94

8 Concluding Remarks 101 A Supplementary Material for Chapter 7 103 A.1 Derivation of the expressions for the transmittance and re-flectance . . . 103

CONTENTS xi

### List of Figures

2.1 Optical conductivity of graphene . . . 16

3.1 Dielectric-metal interface. . . 18

3.2 Dispersion relation of TM SPPs at a dielectric-metal interface (zero damping). . . 21

3.3 Dispersion relation of TM SPPs in air/Ag and SiO2/Ag inter-faces (finite damping). . . 23

3.4 *<{q} and ={q} of TM SPPs at an air/Ag interface. . . 24*

3.5 Propagation lengths of SPPs at dielectric/metal interfaces. . . 27

3.6 Penetration depths of the EM fields due to SPPs at an inter-face between air and silver. . . 28

3.7 Double DMD/MDM interface. . . 30

3.8 Dispersion relation of TM SPPs in a thin film. . . 34

3.9 Electric field profile of SPPs in a double interface: symmetric and antisymmetric modes . . . 35

3.10 Experimentally obtained dispersion curve of SPPs in a thin Al film. . . 35

3.11 Propagation length of LRSPPs and SRSPPs in Ag thin films. 37 4.1 Graphene between two dielectric media . . . 40

4.2 Dispersion relation of TM GSPs. . . 43

4.3 *Dispersion relation of TM GSPs (finite γ 6= 0). . . .* 44

4.4 Electric (vector) field due to TM GSPs. . . 50

4.5 Double-layer graphene structure . . . 53

xiv LIST OF FIGURES

4.7 GSPs’ electric field corresponding to the optical mode . . . 58

4.8 GSPs’ electric field corresponding to the acoustic mode . . . . 59

5.1 Configuration for grating coupling. . . 62

5.2 Diagram of the prism coupling technique. . . 63

5.3 Infrared nano-imaging of GSPs. . . 65

6.1 Metal contact on top of graphene. . . 68

6.2 In-plane electric field due to the contact inhomogeneity. . . 76

6.3 **Intensity plots of the E**2D components. . . 79

6.4 **Electric field lines of E**2D*(x, z).* . . . 80

7.1 Graphene with a spatially-dependent periodic conductivity. . . 82

7.2 Periodic array of graphene ribbons. . . 88

7.3 Unit cell of the periodic structure. . . 89

7.4 *Absorbance, transmittance and reflectance of a p-polarized*
wave through a periodic structure of graphene ribbons. . . 90

7.5 Dependence of the GSP frequency on the electronic density. . 91

7.6 Dependence of the GSP frequency on the periodicity of the system. . . 92

7.7 *Absorbance of a grid of graphene ribbons for varying θ and*
*dg/R ratio. . . .* 93

7.8 Experimental setup of an array of graphene micro-ribbons. . . 94

7.9 *Transmittance change spectrum, −∆T /TCN P* *= 1 − T /TCN P*:
theory and experiment. . . 96

*7.10 Normalized spectra of −∆T for arrays of ribbons with different*
widths: theory and experiment. . . 98
A.1 Relative contribution of different harmonics to the resonances. 106

### List of Acronyms

2D two-dimensional

2DEG two-dimensional electron gas AFM atomic force microscope ATR attenuated total reflection CNP charge neutral point

EELS electron energy loss spectroscopy EM electromagnetic

GSP graphene surface plasmon-polariton IR infrared

LDOS local density of states

LRSPP long-range surface plasmon-polariton LSP localized surface plasmon

SNOM scanning near-field optical microscope SPP surface plasmon-polariton

SRSPP short-range surface plasmon-polariton TE transverse electric

xvi CHAPTER 0. LIST OF ACRONYMS THz terahertz

### Chapter 1

### Introduction

### 1.1

### Context

Despite the recent burst of interest in plasmonics, plasmon-related effects can be traced back to the turn of the twentieth century through the works of A. Sommerfeld and J. Zenneck on the propagation of electromagnetic waves along the surface of a conductor [1, 2]. Concurrently, in 1902, R. H. Wood reported the observation of anomalous intensity drops in the spectrum of visible light diffracted by a metallic grating, which became known as Wood’s anomalies [3]. However, Wood was unable to came up with an interpretation for this phenomenon. The first effort to provide a theoretical explanation was conducted by Lord Rayleigh [4], albeit with limited success, followed by the works of Fano a few decades later [5], which led to subsequent improvements [6]. Some of these breakthroughs took place during the 1950s and 1960s [7, 8], along with the development of the concept of surface plasmon-polariton and its excitation using fast electrons [9, 10] and via prism coupling [11, 12, 13]. Surface plasmon-polaritons (SPPs) are electromagnetic surface waves cou-pled to collective excitations of the conduction electrons, propagating along the interface between a dielectric and a conductor. When this coupled exci-tations occur in metallic nanostructures, the corresponding non-propagating plasmon-polaritons are generally coined as localized surface plasmons (LSPs). Notwithstanding, modern plasmonics as we know it emerged in the turn

1. INTRODUCTION

of the 21st century with the observation, by T. W. Ebbesen et al, of an “extraordinary optical transmission through sub-wavelength hole arrays” in a periodically patterned metal film [14]. Shortly after, a theoretical account for the referred experiment was developed invoking the role SPPs [15]. One notable feature of SPPs (and LSPs) modes is that their momentum is larger than light’s momentum corresponding to photons with the same frequency [16]. As a consequence, these are bound modes whose fields decay exponen-tially away from the interface, exhibiting subwavelength confinement and field enhancement (which can be several orders of magnitude) beyond the reach of conventional optics [16, 17, 18]. Thus, plasmonics opened up the possibil-ity for manipulating light and control light-matter interactions at scales well below the diffraction limit, being one of the most promising research topics in the field of nanophotonics and also an important ingredient in the design and implementation of metamaterials [19, 20, 21].

Nowadays, plasmonics plays a leading role towards the miniaturization of photonic structures and circuitry, along with their integration with cur-rent semiconductor technologies [22]. As far as telecommunications and/or information processing are concerned, photonics offers high speeds and large bandwidths, but this comes with the cost of bulky components (in com-parison to chip-based nanoelectrics); on the other hand, although electronics provides miniaturization and good carrying capacities, its ability to deal with huge amounts of information is limited by the number of connections, result-ing in transmission bottlenecks. Therefore, the hybrid nature of SPPs (beresult-ing half-light, half-matter bosonic quasiparticles, i.e. polaritons) makes them an attractive route to close the gap between optical and electronic circuits, by combining the advantages of both ”worlds”.

The revival of the field over the past decade was, to a large extent, due to rapid development of nanoscale fabrication techniques and experimen-tal tools, together with the implementation of powerful numerical modelling based on full-wave electromagnetic simulations. These triggered the emer-gence of a plethora of exciting applications (which are often strong motivators by themselves), such as spectroscopy and biochemical sensing [19, 23, 24], op-tical tweezers [25, 26], photovoltaics and energy harvesting [27, 28],

1.1. CONTEXT P. A. D. Gon¸calves

tics and nanomedicine [29, 30, 31], SPP-based amplifiers and lasers [32, 33], Fourier and transformation optics [34, 35], etc. Yet, the field of plasmon-ics is far from being exhausted and continues to thrive. Recently, special attention has been given to forefront research topics including ultrafast plas-monics [36], non-linear phenomena with SPPs [37] and quantum plasplas-monics [38]. The latter studies the quantum properties of SPPs, setting up novel pathways to investigate new fundamental physics and to fuel the prospec-tion for plasmonic devices operating at the quantum regime [39, 40]. Several quantum optics experiments with SPPs have been reported [41, 42, 43, 44].

In the present work, we are concerned with graphene as a plasmonic ma-terial – graphene plasmonics [45]. Discovered in 2004 [46], graphene – a two-dimensional (2D) crystal made up of carbon atoms arranged in a honey-comb lattice – has been one of the hottest topics in condensed matter physics, owing to its remarkable electronic, mechanical and optical properties [47, 48]. As in the case of plasmonics, the number of publications on graphene physics has escalated during the past decade. However, the two fields have evolved quite independently up until recently.

Doped graphene is capable of sustaining SPPs [49, 50, 51, 52, 53, 54, 55],
which can be actively controlled and tuned through chemical doping or
elec-trical gating almost in real time. This contrasts with conventional
metal-based plasmonics, where the tunability is usually limited. Furthermore,
graphene surface plasmon-polaritons (GSPs) enable higher levels of spatial
confinement and suffer from relatively low losses when compared with
tradi-tional plasmonic materials, thereby making graphene an appealing candidate
for nanoplasmonics and nanophotonics. Additionally, although the frequency
of GSPs scales with momentum as√*q like in classic 2DEGs (two-dimensional*

electron gases), the GSP frequency is proportional to the electronic density
*as n1/4 _{e}*

*, which is specific of graphene (for 2DEG, a n1/2*scaling is observed instead). This is a direct consequence of the unique electronic properties of graphene, whose electrons behave like relativistic Dirac fermions following a linear dispersion (at low energies in the vicinity of the Dirac point) [48]. An-other peculiarity of graphene is its ability to support transverse electric (TE) SPP modes [56], which do not occur in ordinary metal/dielectric structures

_{e}1. INTRODUCTION

[16].

The frequencies of transverse magnetic (TM) GSP typically lie between the terahertz (THz) and mid-infrared regions of the electromagnetic spec-trum. While the THz spectral region remains relatively unexplored, THz photonics is becoming an active field of research over the last few years [57]. Here too, graphene plasmonics may contribute to the development of the aforementioned subject [58, 59].

Research on graphene plasmonics is intense and likely to remain one of the hottest topics in nanophotonics in the forthcoming years. In addition, the exploration of the unique properties of graphene surface plasmons may lead to a new gold rush with high impact both in fundamental science as well as in technology and industry, ultimately leading to the appearance of the next generation of devices with tailored optoelectronic properties.

### 1.2

### Structure of this thesis

This thesis is organised as follows. In Chapter 2 we lay down the theoretical foundations of classical electrodynamics and solid state physics, accompanied with a concise introduction to graphene with particular attention given to the description of its dynamical conductivity. Then, in Chapter 3 we review the fundamental properties of SPPs in conventional metal-dielectric interfaces, while introducing key concepts in plasmonics. The study of graphene surface plasmons, which is the main focus of this dissertation, begins in Chapter 4. Here, we investigate the general properties of GSPs in extended monolayer graphene sandwiched between two insulating media and also in double-layer graphene (where the graphene sheets are separated by a core dielectric layer), including the calculation of the corresponding dispersion relations and the computation and plotting of the full vectorial fields in both cases. Along the way, some analytical results in closed-form are obtained by employing some approximations. In Chapter 5 we give some examples of the most pop-ular techniques to bypass the missing momentum (between light and SPPs) and effectively excite GSPs. Chapter 6 is devoted to the investigation of the assisted launching of GSPs in continuous graphene by resonant light

1.2. STRUCTURE OF THIS THESIS P. A. D. Gon¸calves

impinging on an infinitely long metal contact localized on top of graphene, thereby making the stripe behave as a dipole antenna. Finally, in Chapter 7, we present an extensive and detailed study of the coupling of free prop-agating electromagnetic radiation to (localized) GSPs in graphene ribbons, namely in a periodic system formed by a set of graphene micro-ribbons akin to a diffraction grating. After building the theoretical framework, we com-pare our analytical results against experimental data in order to validate our model.

In this work we have covered many aspects of the physics governing the properties and the nature of SPPs supported by graphene. A number of prob-lems were addressed, ranging from rather generic systems to particular, well-defined problems involving GSPs in graphene-based structures. Throughout this thesis we tried to present the solutions to the above-mentioned problems with a fair amount of detail (yet without prejudice to the readability of the text), with the aim to make this document as self-contained as possible. Spe-cial attention was also given to the interpretation and clarity of the results. Therefore, we hope that this dissertation will not only serve as a springboard for any newcomer in graphene nanoplasmonics, but also a valuable tool for the advanced researcher to keep at hand.

1. INTRODUCTION

### Chapter 2

### Electromagnetic Properties of

### Solids

In this Chapter, we lay the foundations which will constitute the framework of the work developed in later Chapters. Here, we shall provide a brief overview on elementary concepts in classical electromagnetism and condensed matter physics.

### 2.1

### Classical Electrodynamics

Nowadays, the quest for a unified theory, commonly known as “Theory of Everything”, remains the Holy Grail of Theoretical Physics. The first step towards this end was taken by James Clerk Maxwell, in 1864, with the publi-cation of his famous article entitled “A Dynamical Theory of the Electromag-netic Field” [60]. By unifying electricity and magnetism, Maxwell headed one of the greatest scientific achievements of the 19th century. In fact, classical electrodynamics can be regarded as the first (classical) unified field theory. Today, within the standard model, classical electromagnetism corresponds to a limit of quantum electrodynamics (QED) [61], dubbed by Richard Feyn-mann as the “jewel of physics” owing to the level of agreement between its predictions and experiment. Still, at macroscopic and mesoscopic scales, pro-vided that the number of photons is large and that momentum and energy

2. ELECTROMAGNETIC PROPERTIES OF SOLIDS

transfers are small, the classical formalism often suffices [62]. This regime is satisfied throughout this work.

### 2.1.1

### Maxwell’s equations

In the scope of Maxwell’s classical electrodynamics, light is described as an electromagnetic wave in the form of a three-dimensional electromagnetic field. Within this framework, light-matter interactions are governed by Maxwell’s equations. In SI units, the macroscopic Maxwell’s equations read [62]

* ∇ · D = ρ ,* (2.1)

**∇ × H =**

**∂D***∂t*

*(2.2)*

**+ J ,****∇ × E = −**

**∂B***∂t*

*,*(2.3)

*(2.4)*

**∇ · B = 0 ,****where E ≡ E(r, t) denotes the electric field, D ≡ D(r, t) the electric *** dis-placement, H ≡ H(r, t) the magnetic field and B ≡ B(r, t) the magnetic*
induction1

_{. In turn, ρ ≡ ρ(r, t) and J ≡ J(r, t) refer to the (free) charge}density and current density, respectively, satisfying the continuity equation (charge conservation)

*∂ρ*

*∂t* * + ∇ · J = 0 .* (2.5)

It should be noted that in the case of graphene (or a 2DEG), lying in a

*z = const. plane, we have*

*ρ = ρ*2D*δ(z)* and **J = J**2D*δ(z) ,* (2.6)

at a given time. Limiting ourselves to media that are linear, uniform and isotropic, and also non-magnetic, one can prescribe the following constitutive

1_{Remark: we will refer to B as being the “magnetic field” multiple times throughout}

this work, though this is technically inaccurate. 8

2.1. CLASSICAL ELECTRODYNAMICS P. A. D. Gon¸calves
relations
* D = *0

*(2.7)*

**E ,****H =**1

*µ*0

*(2.8)*

**B ,***where *0 *is the electric permittivity of vacuum and µ*0 its magnetic

*permeabil-ity; these relate to the speed of light in vacuum via c*−2 *= *0*µ*0. The quantity
* represents the relative permittivity or dielectric constant. Another *

impor-tant constitutive relation, for conducting materials, is the generalized Ohm’s law,

* J = σE .* (2.9)

*with σ being a frequency-dependent conductivity. We note that, in general,*
the linear relationships expressed through equations (2.7) and (2.9) should
be understood as
* D(r, t) = *0
Z

*0*

**dr***dt*0

*0*

**(r − r***, t − t*0

**)E(r**0

*, t*0

*) ,*(2.10)

*Z*

**J(r, t) =***0*

**dr***dt*0

*0*

**σ(r − r***, t − t*0

**)E(r**0

*, t*0

*) ,*(2.11)

*where stands now as a function – dielectric function. Equations (2.10) and*

**(2.11) simply state that the value of D and J at a given position r and time**

* t, depends on the value of E at all positions r*0

*and times t*0

*< t (to preserve*

* causality) via the response functions (r − r*0

*, t − t*0

*0*

**) and σ(r − r***, t − t*0), respectively. Consequently, this accounts for both temporal dispersion and non-local effects in space (spatial dispersion), meaning that the optical re-sponse is frequency- and momentum-dependent. While the former is usually evident, the latter can be safely neglected in most cases (as long as the cor-responding wavelength is larger than the electron’s mean free path).

In Fourier space, the above equations translate to

* D(r, ω) = *0

*(2.12)*

**(r, ω)E(r, ω) ,**2. ELECTROMAGNETIC PROPERTIES OF SOLIDS

*in the long-wavelength limit (q → 0), i.e. local response. Also, the Fourier*
transform

**E(r, ω) =**

Z

* E(r, t)e−iωtdt ,* (2.14)

is implicit, and similar relations apply for the remaining fields.

Furthermore, notice that in the absence of free charges and currents (as in free space or dielectric media), Maxwell’s equations reduce to

* ∇ · E = 0 ,* (2.15)

**∇ × B =**

*c*2

**∂E***∂t*

*,*(2.16)

**∇ × E = −**

**∂B***∂t*

*,*(2.17)

*(2.18)*

**∇ · B = 0 .**In addition, expressions (2.16) and (2.17) can be written as
**∇ × B = −i**ω

*c*2* E ,* (2.19)

* ∇ × E = iωB ,* (2.20)

(2.21)
*where a harmonic time dependence in the form of e−iωt* is assumed [or,
equiv-alently, allowing a decomposition of the fields in terms of a plane-wave
ex-pansion – cf. equation (2.14)].

To conclude, let us just mention that by combining the curl equations (2.16) and (2.17), one arrives at the following Helmholtz equations for the electric and magnetic fields,

∇2_{−} 1
*v*2
*∂*2
*∂t*2
!
**E(r, t)*** B(r, t)*

*= 0 ,*(2.22)

which is a wave equation describing an electromagnetic wave travelling at

*v = c/*√*.*

2.2. DRUDE MODEL P. A. D. Gon¸calves

### 2.1.2

### Boundary conditions

Up to now we have considered electromagnetic fields in homogeneous media. Whenever the physical system under consideration involves more than one material, we must introduce the appropriate boundary conditions at each interface. These are obtained by applying the divergence theorem and Stoke’s theorem to Maxwell’s equations, yielding [62]

**n · (D**1**− D**2*) = ρs* *,* (2.23)

**n · (B**_{1}**− B**2*) = 0 ,* (2.24)

**n × (B**1**− B**2*) = µ*0**J***s* *,* (2.25)

**n × (E**1 **− E**2*) = 0 ,* (2.26)

**where n is a unit vector normal to the interface (pointing from medium 2 to**
*medium 1), whereas ρs* **and J***s* are the (idealized) surface charge and surface
current densities on the boundary, respectively.

### 2.2

### Drude Model

Shortly after J. J. Thomson’s discovery of the electron, Paul Drude came up with a model for the description of the electrical and thermal conduction in metals, borrowing the basic ideas of the successful kinetic theory of gases [63]. The Drude model attempts to explain the elementary properties of met-als by regarding a metal as being essentially a free electron gas. Within this description, the loosely bound conduction electrons form an electron gas mov-ing against a lattice of widely spaced, small ionic cores (encompassmov-ing both the nucleus and the tightly bound core electrons) in response to an applied electromagnetic field. The only interaction is via (instantaneous) collisions of electrons with the fixed ions, which occur with probability per unit time

*τ*−1*, where τ is a phenomenological parameter known as the relaxation time.*
Therefore, the equation of motion for an electron of the metal subjected to

2. ELECTROMAGNETIC PROPERTIES OF SOLIDS

* an external electric field E(t) = E*0

*e−iωt*, becomes [64]

**dp(t)***dt* = −

**p(t)**

*τ* * − eE(t) ,* (2.27)

*where e is the elementary charge. We are now looking for a steady-state*
solution exhibiting the same harmonic time dependence of the driving field,
so that the Fourier transform of equation (2.27) yields

**−iωp(ω) = −****p(ω)**

*τ* * − eE(ω) ,* (2.28)

whose solution is

**p(ω) =****eE(ω)**

*iω − τ*−1 *.* (2.29)

*Moreover, notice that the current density due to ne*electrons per unit volume,
**travelling with net velocity v, is J = −en**e**v. Hence, one can write**

**J(ω) = −**ene**p(ω)***me*
= *e*
2_{n}*e*
*me*
1
*γ − iω E(ω) ,* (2.30)

*where me* is the mass of the electron and we have introduced the scattering
*rate, defined as γ = τ*−1. By comparing the result (2.30) with the relation
(2.9), the expression for the optical conductivity can be determined

*σ(ω) =* *e*
2_{n}

*e/me*

*γ − iω* *.* (2.31)

It will be useful for what follows to note that the conductivity and the dielectric function are linked through the following relationship2

*(ω) = 1 + iσ(ω)*
0*ω*
*,* (2.32)
allowing us to write
*(ω) = 1 −* *ω*
2
*p*
*ω*2_{+ iγω}*,* (2.33)

2_{This can be readily shown by working through Maxwell’s equation using the }

consti-tutive relation (2.30) [64].

2.3. GRAPHENE FOR PLASMONICS P. A. D. Gon¸calves

*where ω*2

*p* = *e*

2_{n}*e*

*me*0 denotes the plasma frequency of the free electron gas.

Despite its simplicity, the Drude model provides fairly good results for many metals (specially alkali metals) in the red and infrared region, where their optical properties are frequently dominated by the role of conduction elec-trons – intraband transitions. For noble metals, it fails to a great extent due to the onset of interband transitions in the visible and ultraviolet re-gions, and to other details of the bandstructure. These interband transitions can be accounted, while maintaining the classical picture, by adding a res-onant contribution (whose resres-onant frequency corresponds to the transition energy) to the equation of motion, leading to a dielectric function containing a Lorentz-oscillator term.

Nevertheless, a fully and accurate description of the physics governing the optical response of metals requires a quantum mechanical formulation. Still, this is often circumvented by employing clever effective/phenomenological parameters and/or extra terms ”by hand”.

### 2.3

### Graphene for Plasmonics

Graphene is a two-dimensional allotrope of carbon, where the carbon atoms are arranged in a honeycomb lattice. Being one-atom-thick, it can be re-garded as a truly 2D material. Since its discovery in 2004 [46], graphene has been capitalizing a lot of the scientific community’s atention due to its remarkable properties: it is stronger than steel and harder than diamond, but also flexible [65]; it exhibits an extremely large thermal conductivity [66] and sustains high current densities; its charge carriers are massless Dirac fermions obeying a Dirac-like relativistic equation, showing ballistic transport with huge electronic mobilities [67] even at room temperature; and the list goes on [47]. Owing to these unique properties, graphene has been dubbed a “wonder material ”.

*Graphene’s structural integrity is a direct consequence of the σ-bonds*
between its carbon atoms. Three out of its four valence electrons (belonging
*to 2s, 2px* *and 2py* *orbitals) form hybridized sp*2 orbitals that make up the

2. ELECTROMAGNETIC PROPERTIES OF SOLIDS

*σ-bonds, resulting in a trigonal planar structure where each carbon atom is*

*covalently bonded to three neighbouring atoms via 1.42 Å long σ-bonds. The*
*remaining electron contributes to the 2pz* orbital, which is perpendicular to
*the sp*2 *orbitals’ plane. The former can further bind with another 2pz* orbital
*from a neighbour carbon atom, leading to the formation of a π-bond. Since*
the unit cell contains two atoms, each contributing with one electron from
*the corresponding 2pz* *orbital, graphene has a half-filled π band. Most of the*
electron dynamics and optical properties of graphene are determined by the
*nature of these π-bonds.*

The low-energy physics of graphene takes place in the vicinity of the Dirac
points (where the filled valence band touches the empty conduction band,
for undoped, pristine graphene). Here, the spectrum of the Dirac fermions
*is linear, following E(k) = ~vFk with vF* ≈ _{300}*c* = 106 m/s [48]. This makes
graphene a suitable platform for relativistic tabletop experiments.

In this work, we shall focus on graphene as being a plasmonic material. As far as graphene plasmonics is concerned, all we need to describe its elec-tromagnetic properties and light-matter interactions is encompassed within graphene’s optical conductivity. Thus, further details on graphene will be overlooked. For a detailed treatment of graphene physics, please refer to [47, 48, 68].

### 2.3.1

### Optical conductivity of graphene

Graphene’s optical conductivity plays a key role in graphene optics and plas-monics. This important physical quantity can be split into two distinct con-tributions: one describing intraband transitions and another accounting for interband transitions, that is

*σg(ω) = σ*intra*(ω) + σ*inter*(ω) .* (2.34)

In writing the last expression it is implicit that we will ignore spatial dis-persion (i.e. non-local effects) henceforth. An analytical expression for the dynamical conductivity of graphene can be obtained under the random phase

2.3. GRAPHENE FOR PLASMONICS P. A. D. Gon¸calves

approximation (RPA) or via Kubo’s formula [69, 70, 71, 72, 73], namely

*σ*intra*(ω) =*
*σ*0
*π*
4
*~γ − i~ω*
h
*EF* *+ 2kBT ln*
*1 + e−EF/kBT*i _{,}_{(2.35)}

*characterizing intraband processes, where σ*0 *= e*2*/(4~), kB* is Boltzmann’s
*constant and EF* *≈ |µ|, while for interband transitions we have*

*σ*inter*(ω) = σ*0
"
*G(~ω/2) + i4~ω*
*π*
Z ∞
0
*dEG(E) − G(~ω/2)*
*(~ω)*2* _{− 4E}*2
#

*,*(2.36) with

*G(x) =*sinh

_{x}*kBT*cosh

_{E}*F*

*kBT*+ cosh

_{x}*kBT*

*.*(2.37)

*At zero temperature, or at least as long as the condition EF* * kBT is*
verified, the above equations reduce to

*σ*intra*(ω) =*
*σ*0
*π*
*4EF*
*~γ − i~ω*
*,* (2.38)
*σ*inter*(ω) = σ*0
"
*Θ(~ω − 2EF*) + *i*
*π*ln
*~ω − 2EF*
*~ω + 2EF*
#
*,* (2.39)

*where Θ(x) stands for the Heaviside step function. Notice that for 2EF* *> ~ω*
*and EF* * ~ω, the term describing interband transitions gives a negligible*
contribution – Pauli blocking. Therefore, we note that for frequencies in the
terahertz (THz) and mid-IR spectral region – the regime that we are
inter-ested in this work –, at room temperature and under typical doping levels,
graphene’s optical conductivity is dominated by term describing intraband
electronic processes, following the Drude-like expression

*σg(ω) ≈*

*σ*0
*π*

*4EF*

*~γ − i~ω* *,* (2.40)

with good accuracy. The results for the conductivity of graphene are sum-marized in figure 2.1.

2. ELECTROMAGNETIC PROPERTIES OF SOLIDS 0 0.02 0.04 0.06 0.08 0.1 0 25 50 75 100 125 Re{σ(ω)}, RPA Im{σ(ω)}, RPA Re{σ(ω)}, Drude Im{σ(ω)}, Drude 0 0.5 1 1.5 2 2.5 3 3.5 -2 -1.5 -1 -0.5 0 0.5 1 1.5 2 2.5

### intraband

### int

### er

### ba

### nd

### a)

### b)

### c)

Figure 2.1: Optical conductivity of graphene: a) real and imaginary parts of the
conductivity computed using the full local-RPA expression [equations (2.35) and
*(2.36)] at T = 300 K (continuous) and at T = 0 K (dashed); b) graphene’s optical*
conductivity in the THz regime, obtained via RPA (continuous) and using Drude’s
expression (2.40) (dashed); c) schematic illustration of the transition processes in
*doped graphene. Parameters: EF* *= 0.3 eV and ~γ = 3.7 meV.*

### Chapter 3

### Surface Plasmon Polaritons at

### Dielectric-Metal Interfaces

Before jumping to graphene plasmonics, it is instructive to begin our study with the well known surface plasmon-polaritons (SPPs) at dielectric-metal interfaces. In this chapter, we will introduce the basic concepts in plasmonics and see how the main features of SPPs arise from the formalism of classical electrodynamics reviewed in the previous Chapter.

### 3.1

### Single Dielectric-Metal Interface

In order to get acquainted with surface plasmon-polaritons, we begin our
investigation by considering the simplest system capable of supporting SPPs.
This corresponds to the case of a single (planar) interface between a dielectric
and a metal. For our convenience, we shall assume that both media are
*semi-infinite, with the dielectric occupying the half-region defined by z < 0 and*
*the metal occupying the half-region where z > 0, as depicted in figure 3.1.*
**Additionally, the system is isotropic along the ˆy direction.**

The dielectric medium is characterized by a real and positive dielectric
*constant, *1, whereas the electromagnetic properties of the metal will be

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

### Metal

### Dielectric

Figure 3.1: Schematic representation of a surface plasmon-polariton at an
inter-face between a dielectric and a metal. The field profile is shown qualitatively for
guidance.
2*(ω), of the form*
2*(ω) = 1 −*
*ω*2
*p*
*ω*2_{+ iωγ}*.* (3.1)

Recall that equation (3.1) is just the dielectric function of the metal within
the free electron gas model [cf. equation (2.33)]. Furthermore, for the sake
*of simplicity, we assume that both *1 *and *2*(ω) are isotropic – homogeneous*

and isotropic media.

The electromagnetic field due to a SPP can be obtained from the solution of Maxwell’s equations, in each medium, in the form of a propagating surface electromagnetic wave which is confined to the whereabouts of the interface, and whose fields decay exponentially along the direction perpendicular to the interface (see, for instance, figure 3.1).

### 3.1.1

### Dispersion relation

Let us first consider transverse magnetic (TM) solutions. These can be writ-ten as

**E***j (r, t) = (Ej,xx + E*

**ˆ**

*j,z*

**ˆ**

**z) e**−κj|z|ei(qx−ωt)*,*(3.2)

**B***j(r, t) = Bj,y y e*

**ˆ**

*−κj|z|*

_{e}i(qx−ωt)

_{,}_{(3.3)}

*where the index j = 1, 2 identifies the medium as in figure 3.1. Inserting*
equations (3.2) and (3.3) into Maxwell’s equations (while assuming that the

3.1. SINGLE DIELECTRIC-METAL INTERFACE P. A. D. Gon¸calves

materials are non-magnetic)

**∇ × E***j* = −
**∂B**j*∂t* *,* (3.4)
**∇ × Bj** = *j*
*c*2
**∂E**j*∂t* *,* (3.5)
yields
*Bj,y* =
*ωj*
*c*2_{q}Ej,z*,* (3.6)
*Bj,y* *= −i sgn(z)*
*ωj*
*c*2_{κ}*j*
*Ej,x* *,* (3.7)
*Ej,x* *= −i sgn(z)*
*κj*
*q* *Ej,z* *,* (3.8)
*κj* =
q
*q*2_{− }*jω*2*/c*2*.* (3.9)

The boundary conditions of the problem require the continuity of the
tangential components (relative to the interface) of the electric and magnetic
*fields across the interface (i.e. at z = 0),*

*E1,x* *= E2,x* *,* (3.10)

*B1,y* *= B2,y* *,* (3.11)

*(note that for non-magnetic media H1,y* *= H2,y* *⇔ B1,y* *= B2,y*). Writing the

amplitudes of the magnetic field in terms of the corresponding electric field’s amplitudes in the second boundary condition, using equation (3.7), we arrive at the following pair of equations:

*E1,x* *= E2,x* *,* (3.12)
1
*κ*1
*E1,x* = −
2*(ω)*
*κ*2
*E2,x* *.* (3.13)

The linear system composed by equations (3.12) and (3.13) has a non-trivial
solution if
1
*κ*1*(q, ω)*
+ 2*(ω)*
*κ*2*(q, ω)*
*= 0 ,* (3.14)

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

from which we obtain the dispersion relation for TM surface plasmon-polaritons
at a dielectric-metal interface. Note that in equation (3.14) we emphasized
*the fact that κ1,2* depends on the frequency as well as on the wavevector in

accordance to equation (3.9). Moreover, in order to have a confined
*electro-magnetic surface wave, it follows from equation (3.14) that if *1 *> 0, then*

*we must have <{*2*(ω)} < 0 [since we need to meet the requirement that*

*<{κ1,2} > 0; see equations (3.2) and (3.3)]. This means that SPPs can only*

exist at interfaces between materials whose (real parts of the) dielectric per-mittivities have opposite signs, such as an interface between an insulator and a metal.

*We can write a more explicit relation for the SPPs’ wavevector, qSP P* , as a

function of the frequency, by subtituting equation (3.9) into equation (3.14),
obtaining
*qSP P* =
*ω*
*c*
v
u
u
t
12*(ω)*
1*+ *2*(ω)*
*.* (3.15)

*We stress that equation (3.15) remains valid even for *2*(ω) with non-zero*

imaginary part, that is, for metals with damping. To better illustrate this result, we shall analyse separately the cases with and without attenuation.

*Zero damping (γ = 0)*

In the case of a lossless conductor, its corresponding Drude’s dielectric func-tion takes the simplified form

2*(ω) = 1 −*
*ω*2

*p*

*ω*2 *.* (3.16)

Figure 3.2 shows the dispersion relation obtained from inserting equation
(3.16) into equation (3.15). The continuous curves represent the real part of
the plasmon’s wavevector and the dashed green curve its imaginary part. It is
*clear that whenever the value of q is a pure imaginary number, the existence of*
propagating modes is forbidden. In figure 3.2, this corresponds to the region
between the two horizontal dashed-dotted lines. Outside this region, we can
identify two kinds of fundamentally different plasmons: bulk plasmons (red

3.1. SINGLE DIELECTRIC-METAL INTERFACE P. A. D. Gon¸calves
0 0.5 1 1.5 2 2.5 3 3.5 4
q c/ω_{p}
0
0.25
0.5
0.75
1
1.25
1.5
Frequency
(ω/ω
p
)
Light
SPPs
Bulk PPs

Figure 3.2: Dispersion relation of TM SPPs at an interface between air and a
Drude metal without damping. We can identify essentially three different regions:
an upper branch with radiative modes (red curve); a lower branch with bound
*SPPs modes (blue curve); and an intermediate region, with <{q} = 0, where*
propagation is forbidden (green dashed curve).

curve) and surface plasmon-polaritons (blue curve). The former consists in
collective oscillations of the free electrons within the metal (also called volume
plasmons), while the latter corresponds to bound excitations confined at the
interface. In addition, in the upper branch of the dispersion relation relative
*to bulk plasmons, we have ω > ωp*, so that radiation propagates through
*metal - radiative modes - with q being real and κj* *→ iκj*. On the other
*hand, since SPPs correspond to bound modes with both q and κj* real, its
dispersion curve must lie to the right of the light line in the dielectric (yellow
line). Consequently, SPPs cannot be readily excited simply by impinging
light onto the system, so that one has to come up with a mechanism capable
of coupling light to surface plasmons. Examples of such techniques are prism
and grating coupling, which will be described in more detail in Chapter 5.

Before moving on to the discussion of the case with a real (lossy) metal, let us take a closer look at the behaviour of SPPs in two limiting cases, those

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

of small and large wavevectors. In the regime of small wavevectors, the SPPs dispersion curve is close to the light line, and the SPP resembles an inci-dent light wave tangent to the interface – Sommerfeld-Zenneck wave. Thus,

*κ*1 1 [cf. equation (3.9)] and the electromagnetic field is poorly confined,

penetrating deep inside the dielectric. Conversely, for large wavevectors, it
is apparent from figure 3.2 that the SPPs dispersion curve approaches a
*lim-iting frequency as q → ∞. This frequency can be obtained from equation*
*(3.15) by setting *1*+ *2*(ω) = 0, yielding*
*ωsp* =
*ωp*
√
*1 + *1
*,* (3.17)

which is known as the surface plasmon frequency and corresponds to the
lower horizontal line in figure 3.2. Note, however, that in this regime the
*group velocity vg* = *∂ω _{∂q}* → 0. Therefore this is a dispersionless mode with an
electrostatic character, dubbed a surface plasmon.

*Finite damping (γ 6= 0)*

In real metals, there is often a miscellania of damping mechanisms which
contribute to the attenuation of SPPs, ranging from electron-electron
inter-actions to impurity and lattice scattering, just to mention a few. Within the
framework of the Drude model, one attemps to account for all these
*phenom-ena by introducing a phenomenological parameter, γ, as in equation (3.1).*
Nevertheless, although the model captures fairly well the dominant features
of noble metals at low frequencies, it fails (to a significant extent) with the
onset of interband transitions at higher frequencies. In order to avoid further
complications, we shall use the actual values of the dielectric function taken
from experiments. In figures 3.3 and 3.4 is plotted the dispersion relation of
SPPs using experimental data obtained from Ref. [74]. The most striking
feature is that in this case there is a finite, maximum allowed wave vector
for the SPPs, in contrast with the previous undamped case (compare, for
instance, figures 3.2 and 3.3). This not only sets up a lower bound for the
*SPPs wavelength, given by λSP P* *= 2π/<{q}, but also limits the degree of*

3.1. SINGLE DIELECTRIC-METAL INTERFACE P. A. D. Gon¸calves
0 20 40 60 80 100
q(µm-1)
0
2
4
6
8
Frequency
(2
π
·PHz)
Light air/Ag
Light SiO_{2}/Ag
SPPs @ air/Ag
SPPs @ SiO_{2}/Ag

Figure 3.3: Dispersion relation of TM SPPs in air/Ag (blue) and SiO2/Ag (red)

interfaces, where we have used experimental data from Ref. [74] to account for
silver’s dielectric function. Owing to damping, the wavevector of the bounded
*SPPs modes is now limited to a maximum value at ωsp* (dotted lines).

*confinement of the mode. Additionally, due to the non-vanishing γ, we now*
have the more general situation where the dielectric function of the
*conduc-tor is a complex-valued function, and, therefore, so it is q, as illustrated in*
figure 3.4. Thus, the SPPs will be attenuated, losing energy as they travel
along the system until they eventually fade away. Finally, note that unlike
*the case of a lossless metal - in which there was a gap, between ωsp* *and ωp*,
where the existence of modes was prohibited (i.e. with a purely imaginary
propagation constant) - we now observe the emergence of quasibound modes
in the aforementioned region.

Before moving on with our study of the basic features of SPPs, let us take a
*step back to analyse the case of a s-polarized, transverse electric (TE) surface*
electromagnetic wave. These modes have the electric field perpendicular to

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES 0 5 10 15 20 25 30 35 q(µm-1) 0 2 4 6 8 Frequency (2 π ·PHz) Light air/Ag Im[q], air/Ag Re[q], air/Ag

Figure 3.4: Dispersion relation with both real and imaginary parts of the
*prop-agation constant, q, of TM SPPs at an interface between air and silver, using*
experimental data from Ref. [74].

the plane of incidence, so that we will be seeking solutions of the type

**E***j (r, t) = Ej,yy e*

**ˆ**

*−κj|z|ei(qx−ωt)*

*,*(3.18)

**B***j (r, t) = (Bj,x*

**ˆ**

**x + B**j,z**ˆ**

**z) e**−κj|z|ei(qx−ωt)*.*(3.19) As before, we substitute the fields (3.19) and (3.18) into Maxwell’s equations (3.4) and (3.5), obtaining

*Bj,z*=

*q*

*ωEj,y*

*,*(3.20)

*Bj,x*

*= −i sgn(z)*

*κj*

*ωEj,y*

*,*(3.21)

*Bj,x*

*= −i sgn(z)*

*κj*

*q*

*Bj,z*

*,*(3.22)

*κj*= q

*q*2

*2*

_{− j}_{ω}*2*

_{/c}

_{.}_{(3.23)}24

3.1. SINGLE DIELECTRIC-METAL INTERFACE P. A. D. Gon¸calves

*The boundary conditions at z = 0, read*

*E1,y* *= E2,y* *,* (3.24)

*B1,x* *= B2,x* *.* (3.25)

Introducing equation (3.21) into the second boundary condition (3.25), and further combining equations (3.24) and (3.25), we arrive at the following condition:

*(κ*1*+ κ*2*)E1,y* *= 0 .* (3.26)

*This condition may be satisfied if either E1,y* *= 0 or κ*1 *+ κ*2 = 0. Note,

*however, that we must have <{κ*1*} > 0 and <{κ*2*} > 0 since we are looking*

for solutions confined to the dielectric-metal interface. Thus, the condition
*given by equation (3.26) can only be fulfilled if E1,y* *= E2,y* = 0, that is, TE

surface plasmon-polaritons cannot exist at interfaces between a dielectric and a conductor.

### 3.1.2

### Propagation length and field confinement

In the above discussion of TM surface plasmon-polaritons, we claimed that
the inherent Ohmic losses in metals render a complex-valued dielectric
*func-tion. Thus, from equation (3.15) it can be seen that q will also be complex,*

*q = q*0*+iq*00, so that the attenuation of the SPPs solutions will be caracterized
*by an exponentially decaying term as exp(−q*00*x).*

*In particular, defining *2*(ω) = *02 *+ i*
00

2 and inserting this into equation

(3.15), we obtain
*q =* *ω*
*c*
v
u
u
t
1*(*02*+ i*002)
1*+ *02 *+ i*002
≈ *ω*
*c*
s
102
1*+ *02
"
*1 + i*1
00
2*/*02
1*+ *02
#*1/2*
*,* (3.27)

*where we have explicitly assumed that |*0_{2}*| > *00

2 (condition satisfied from

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

*the terms of order O ([*00_{2}]2_{). Expanding equation (3.27), yields}

*q ≈* *ω*
*c*
s
102
1*+ *02
"
1 + *i*
2
102
1*+ *02
00_{2}
*(*0
2)2
#
*,* (3.28)

from which we identify

*q*0 = *ω*
*c*
s
102
1*+ *02
and *q*00 = 1
2
*ω*
*c*
102
1*+ *02
!*3/2*
00_{2}
*(*0_{2})2 *.* (3.29)

*Since the electromagnetic field intensity of SPP decreases as exp(−2q*00*x),*

its characteristic propagation length is given by

*LSP P* =
1
*2={q}* ≈
1
*2q*00 =
*c*
*ω*
1*+ *02
102
!*3/2*
*(*0_{2})2
00_{2} *,* (3.30)

**which defines the distance that the SPP travels until its intensity (along ˆx)**

*falls by 1/e. Figure 3.5 shows the propagation lengths for surface *
plasmon-polaritons at air/silver and silica/silver interfaces (blue and red curves,
re-spectively). Note that for wavelengths within the visible region, the
*propaga-tion distances are of the order of a few micrometers up to 100 µm, whereas in*
*the infrared they can reach values between 100 and 1000 µm. Naturally, these*
values depend upon the specific dielectric/metal involved1_{. Additionally, we}

find that the propagation length attains its minimum value as the frequency
*approaches ωsp*, as we had already anticipated in the previous subsection.

One of the most interesting properties of SPPs is their ability to
con-fine the electromagnetic field, in the direction perpendicular to the interface,
down to subwavelength scales beyond the diffraction limit. Since along this
*direction the fields fall off as exp(−κj|z|), we can quantify the ”degree of field*

1_{We further note that even for the very same metal we can come up with different results}

depending on the source of empirical data retrieved from the literature - e.g. compare figures 3.5a and 3.5b, obtained using data taken from Refs. [74] and [75], respectively. The reasons for the discrepancies observed among several experimental data available in the literature are still motif of debate and we shall not enter in such muddy waters.

3.1. SINGLE DIELECTRIC-METAL INTERFACE P. A. D. Gon¸calves
Ener
gy
(eV)
0
1
2
3
4
5
q (μm-1_{)}
0 20 40 60 80
V
acu
um
wavel
ength
(nm)
1,240
619.9
413.3
310
248
L (μm)
10−2 _{10}−1 _{10}0 _{10}1 _{10}2 _{10}3 _{10}4

(a) Left panel: dispersion relation of TM SPPs at air/Ag and SiO2 interfaces (similar to figure 3.3). Right panel:

corresponding propagation lengths. The full curves were
*obtained directly from L = (2={q})*−1, while the
dot-dashed curves were computed using the approximate
ex-pression presented in equation (3.30). The dielectric data
was taken from Ref. [74].

300 600 900 1200 1500 1800
Vacuum wavelength (nm)
10-3
10-2
10-1
100
101
102
103
L
(µ
m)
air/Ag
SiO_{2}/Ag

(b) The same as in figure 3.5a (right panel) but now using the experimental data from Ref. [75].

Figure 3.5: Propagation lengths of SPPs at dielectric/metal interfaces.

*confinement” by introducing the penetration depth, ζ, defined as*

*ζj* =
1

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

*We can obtain an approximate expression for ζ in equation (3.31), by *
sub-stituting equation (3.15) into equation (3.9), from which we arrive to

*ζdiel.* =
*c*
*ω*
v
u
u
t
*|*0
2*| − *1
2
1
and *ζ*metal =
*c*
*ω*
v
u
u
t
*|*0
2*| − *1
*(*0_{2})2 (3.32)

for both the dielectric and the metal, as indicated by the subscripts in (3.32).
*In writing these expressions, we explicitly used the fact that *0_{2}must be
nega-tive in order for SPPs to exist [recall our discussion after equation (3.14)], and
*we have neglected *00_{2}. The behaviour of the penetration depths (also called
attenuation length) of the electromagnetic field due to SPPs as a function of
the corresponding vacuum wavelength is depicted in figure 3.6. In the metal,

300 600 900 1200 1500 1800 Vacuum wavelength (nm) 0 600 1200 1800 2400 3000 3600 4200 Penetrat ion depth (nm) Air Silver 30 SPPs

Figure 3.6: Penetration depths of the EM fields due to SPPs into air (blue curve)
and silver (maroon curve), calculated using the optical constants from Ref. [74].
*Note that we have plotted the penetration into the metal below the ζ = 0 line,*
and notice the different scale in that region. The dot-dashed curves correspond to
the approximate values obtained using expressions (3.32).

the penetration length is roughly constant for wavelengths below the surface plasmon frequency and it can be several orders of magnitude smaller than

3.2. MULTILAYER STRUCTURES P. A. D. Gon¸calves

in the dielectric. In contrast, the penetration depth of the electromagnetic field into the dielectric grows with increasing wavelength. This means that the ability of SPPs to confine the electromagnetic field deteriorates as the wavelength (frequency) increases (decreases).

We end our preliminary discussion of the basic properties of SPPs at single interfaces by noting that while the field confinement is weaker at lower frequencies (as we have just seen), the corresponding propagation length is larger (cf. figure 3.5). Thus, higher field localization comes hand in hand with larger losses. This trade-off between field confinement and propagation length is characteristic of plasmonics.

### 3.2

### Multilayer Structures: Double Interface

Up to now, we have only treated the simplest case of a single flat
dielectric-metal interface. Nevertheless, the landscape encompassing SPPs turns out
to be much richer. The natural next step is to pursue our studies on SPPs
in more complex (but still planar) geometries, such as systems containing
several interfaces. From our previous endeavour, we expect that these
multi-layer structures have the capacity to sustain SPPs modes whenever there is
an interface between a dielectric and a conductor. However, as we shall see
ahead, SPPs in such heterostructures may exhibit interesting phenomena out
of reach of ordinary SPPs at single interfaces. For the sake of clarity and
ped-agogy, as well as historical significance, here we will consider essentially two
different systems: a thin metal film cladded between two semi-infinite
dielec-tric media - dielecdielec-tric/metal/dielecdielec-tric (DMD) structure - and its ”image”,
that being a dielectric layer sandwiched between two semi-infinite metallic
layers - metal/dielectric/metal (MDM) structure. The common denominator
is that both heterostructures can be regarded as three-layer systems with a
double interface. In the case of a thin film, we already antecipated that bound
SPPs solutions should exist at each of its interfaces. The novelty emerges
*when the thickness of the metallic film, d, becomes sufficiently small*2 _{to}

2* _{To be more quantitative, by sufficiently small we mean κ}*
2

*d 1.*

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

Figure 3.7: Schematic representation of a three-layer heterostructure - either DMD
or MDM - capable of supporting surface plasmon-polaritons at each of its
dielec-tric/metal interfaces. For metallic media it is implicit that its corresponding
*di-electric function is frequency-dependent, i.e. m(ω), where the subscript stands for*
*”metal”. The width of the core layer is caracterized by d, and the cladding media*
are assumed to be semi-infinite. In addition, the field of both two non-interacting
surface plasmon-polaritons and a hybridized mode are qualitatively illustrated for
eye guidance.

enable the communication between the electromagnetic fields of the SPPs modes at opposite interfaces. The result of this interaction will be the split-ting of the retarded SPP condition, given by equation (3.15), into a set of two distinct new modes.

### 3.2.1

### Dispersion relation

The procedure to derive the dispersion relation of surface plasmon-polaritons in a double interface will follow, in essence, the same steps as in subsection 3.1.1 for one dielectric-metal interface. The electromagnetic fields in the top and bottom media have the usual form of a TM surface wave

**E***j (r, t) = (Ej,x*

**ˆ**

**x + E**j,z**ˆ**

**z) e**−κj|z|ei(qx−ωt)*,*(3.33)

**B***j (r, t) = Bj,y*

**ˆ**

**y e**−κj|z|ei(qx−ωt)*,*(3.34)

3.2. MULTILAYER STRUCTURES P. A. D. Gon¸calves
with
*Bj,y* =
*ωj*
*c*2_{q}Ej,z*,* (3.35)
*Bj,y* *= −i sgn(z)*
*ωj*
*c*2_{κ}*j*
*Ej,x* *,* (3.36)
*Ej,x= −i sgn(z)*
*κj*
*q* *Ej,z* *,* (3.37)
*κj* =
q
*q*2_{− }*jω*2*/c*2*.* (3.38)

*now for j = 1, 3 only [where z < 0 in region 1 and z > d in region 3* 3
*(see figure 3.7)]. The situation becomes different for medium j = 2 (where*
*0 < z < d). Here, the fields can be described as a superposition of an*
exponentially growing wave with an exponentially decaying wave, of the form

**E**2* (r, t) =*
n

*E*(+)

_{2,x}

**x + E****ˆ**

*(+)*

_{2,z}**ˆz**

*eκ*2

*z*

_{+}

*(−)*

_{E}*2,x*

**ˆ**

*(−)*

**x + E***2,z*

**ˆz**

*e−κ*2

*z*o

_{e}i(qx−ωt)*(3.39)*

_{,}**B**2

**(r, t) =***B*(+)

_{2,y}*eκ*2

*z*(−)

_{+ B}*2,y*

*e*

*−κ*2

*z*

_{y e}

_{ˆ}*i(qx−ωt)*

_{,}_{(3.40)}

satisfying the relations

*B _{2,y}*(+)= −

*ω*2

*c*2

*(+)*

_{q}E*2,z*

*,*(3.41)

*B*(+)

_{2,y}*= iω*2

*c*2

*2*

_{κ}*E*(+)

_{2,x}*,*(3.42)

*B*(−)= −

_{2,y}*ω*2

*c*2

*(−)*

_{q}E*2,z*

*,*(3.43)

*B*(−)

_{2,y}*= −iω*2

*c*2

*2*

_{κ}*E*(−)

_{2,x}*,*(3.44)

*κ*2 = q

*q*2

*2*

_{− }*ω*2

*/c*2

*,*(3.45)

connecting the amplitudes of the magnetic field with the corresponding am-plitudes of the electric field. Since now we have two interfaces, we will need

3_{Note that in the latter we could also have written the z-dependence of the fields in}

*equations (3.33) and (3.34) as e−κ*3*(z−d) _{. As written in the text, the factor e}κ*3

*d*

_{is taken}

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES

*to employ two sets of boundary conditions, one at z = 0,*

*E1,x* *= E*
(+)
*2,x* *+ E*
(−)
*2,x* *,* (3.46)
*B1,y* *= B*
(+)
*2,y* *+ B*
(−)
*2,y* *,* (3.47)

*and the other at z = d,*

*E _{2,x}*(+)

*eκ*2

*z*

*(−)*

_{+ E}*2,xe*

*−κ*2

*z*

_{= E}*3,xe−κ*3

*z*

*,*(3.48)

*B*(+)

_{2,y}*eκ*2

*z*(−)

_{+ B}*2,y*

*e*

*−κ*2

*z*

_{= B}*3,ye−κ*3

*z*

*.*(3.49)

Using expressions (3.35-3.38) and (3.41-3.45), one arrives at the following homogeneous linear system of equations

−1 1 1 0
−1
*κ*1
2
*κ*2 −
2
*κ*2 0
0 *eκ*2*d* * _{e}−κ*2

*d*

*3*

_{−e}−κ*d*0 2

*κ*2

*e*

*κ*2

*d*

_{−}2

*κ*2

*e*

*−κ*2

*d*3

*κ*3

*e*

*−κ*3

*d*

*E1,x*

*E*(+)

_{2,x}*E*(−)

_{2,x}*E3,x*

*= 0 .*(3.50)

The dispersion relation for transverse magnetic SPPs in a double interface is then obtained by solving the condition that the determinant of the matrix in (3.50) must be zero in order to exist a non-trivial solution, yielding

1 + 2*κ*1
1*κ*2
1 + 2*κ*3
3*κ*2
=
1 −2*κ*1
1*κ*2
1 − 2*κ*3
3*κ*2
*e−2κ*2*d* _{.}_{(3.51)}

*This expression must be solved numerically, and it is implicit that κj* ≡

*κj(q, ω) and that j* *≡ j(ω) for j referring to metallic media. Note that*

*in the limit d → ∞ (or κ*2*d 1), corresponding to thick films in DMD*

heterostructures or to thick dielectric cores in MDM heterostructures, we get from equation (3.51) the conditions

1
2
+ *κ*1
*κ*2
= 0 *and/or* 3
2
+*κ*3
*κ*2
*= 0 ,* (3.52)

which are just the decoupled dispersion relations of the individual TM SPPs at each interface [cf. (3.14)].

3.2. MULTILAYER STRUCTURES P. A. D. Gon¸calves

It is interesting to consider the particular case of a symmetrical
envi-ronment, in which the substrate and the superstrate are made of the same
*material, and thus *1 *= *3 *and κ*1 *= κ*3. Under these circumstances, the

dispersion relation (3.51) can be further simplified, and splits into two modes delivered by the following pair of equations:

*ω*+ *: tanh(κ*2*d/2) = −*
2*κ*1
1*κ*2
*,* (3.53)
and
*ω*− *: coth(κ*2*d/2) = −*
2*κ*1
1*κ*2
*,* (3.54)

corresponding to a high-frequency mode and a low-frequency mode, as
indi-cated by the subscripts. In addition, it is also common to encounter these
solutions in literature classified as an odd mode, where the tangential
*com-ponent of the electric field (Ex*) is antisymmetric with respect to the plane

*z = d/2; and an even mode, in which the tangential component of the electric*

*field is symmetric relative to the z = d/2 plane. Figure 3.8 shows the *
disper-sion relation of non-radiative4 SPPs in silver thin films (DMD
heterostruc-tures) free-standing in air, computed using equations (3.53) and (3.54) for
*several different widths. Silver’s dielectric function, *2*(ω), is modeled as a*

free electron gas with negligible damping [see, for instance, equation (3.16)].
From figure 3.8 we see that in the case of the thickest film (orange dot-dashed
line), its dispersion curve consists in two almost decoupled, degenerate modes
(due to the symmetrical environment) and is indistinguishable to the one of
a single air/Ag interface (black curve). However, as the film thickness is
decreased, the evanescent tails of the SPPs in each interface overlap and
hybridize, modifying the (independent) SPP dispersion. This interaction
be-tween the electromagnetic fields on different interfaces act as a perturbation
which removes the degeneracy of the spectrum, splitting the original
*dis-persion relation into two branches, ω*+ *and ω*−, corresponding to modes in

which the component of the electric field along the propagation direction is

4_{We mention that in this geometry the dispersion relation also returns solutions between}

*ωp* and the curves plotted in figure 3.8 (not shown for clarity). These are highly damped,
*short-lived modes [76] (even when γ → 0), so that we shall ignore them onwards.*

3. SURFACE PLASMON POLARITONS AT DIELECTRIC-METAL INTERFACES
0 20 40 60 80 100 120 140
q(µm-1)
0
1
2
3
4
5
6
7
8
9
ω
(eV)
d = 100 nm
d = 50 nm
d = 12 nm
d = 2 nm
ω_{+}
ω_{−}

Figure 3.8: Dispersion relation of TM SPPs in a thin film, namely an air/silver/air
multilayer structure, showing the hybridized, coupled modes for various mettalic
*layer thicknesses, d, indicated in the plot. The black curve represents the *
dis-persion curve of SPPs in a single air/silver interface and the dashed violet line
the dispersion of light in the dielectric. The broken horizontal line indicates the
asymptotic surface plasmon frequency. Here, silver is assumed to be a lossless
*Drude metal with ωp* *= 9.2 eV.*

*an odd and an even function of z − d/2, respectively, as figure 3.9 illustrates.*
Furthermore, for sufficiently thin films, the antisymmetric solution exhibits
*an obvious maxima at frequencies above ωsp* in contrast both to the
symmet-ric solution and to the single-boundary dispersion curve. Recall that for the
*latter, there is a gap between ωspand ωp* where propagation is not allowed (cf.
figure 3.2). Additionally, note that the odd mode approaches the asymptotic
surface plasmon frequency from above, with negative group velocity. On the
other hand, the even mode has the ability to achieve large wavevectors at
*frequencies well below ωsp*, meaning that the corresponding SPP wavelengths
will be extremely short.

The splitting of the SPPs dispersion curve due to the two coupled (bounded) modes in a thin oxydized aluminum film was experimentally demonstrated by